Sintering effects on chemical and physical properties of bioactive ceramics · PDF file...
Embed Size (px)
Transcript of Sintering effects on chemical and physical properties of bioactive ceramics · PDF file...
Journal of Advanced Ceramics 2013, 2(3): 274–284 ISSN 2226-4108 DOI: 10.1007/s40145-013-0072-y CN 10-1154/TQ
Sintering effects on chemical and physical properties of bioactive ceramics
Lukasz WITEKa,b,*, James SMAYa, Nelson R. F. A. SILVAc, Teja GUDAd, Joo L. ONGd, Paulo G. COELHOb,e
aSchool of Chemical Engineering, Oklahoma State University, 423 Engineering North, Stillwater, OK, USA bDepartment of Biomaterials and Biomimetics, New York University, 345 East 24th Street, 804S New York, NY, USA cDepartment of Operative Dentistry, Universidade Federal de Minas Gerais, Pampulha, Belo Horizonte, MG, Brazil dDepartment of Biomedical Engineering, University of Texas San Antonio, One UTSA Circle, San Antonio, TX, USA
eDepartment of Periodontology and Implant Dentistry, College of Dentistry, New York University, 345 East 24th Street, New York, NY, USA
Received: March 01, 2013; Revised: May 16, 2013; Accepted: June 13, 2013 ©The Author(s) 2013. This article is published with open access at Springerlink.com
Abstract: The objective of this study was to characterize the chemical and physical properties of bioactive ceramics prepared from an aqueous paste containing hydroxyapatite (HA) and beta tri-calcium phosphate (β-TCP). Prior to formulating the paste, HA and β-TCP were calcined at 800 ℃ and 975 ℃ (11 h), milled, and blended into 15%/85% HA/β-TCP volume-mixed paste. Fabricated cylindrical rods were subsequently sintered to 900 ℃, 1100 ℃ or 1250 ℃. The sintered specimens were characterized by helium pycnometry, X-ray diffraction (XRD), Fourier transform-infrared (FT-IR), and inductively coupled plasma (ICP) spectroscopy for evaluation of porosity, crystalline phase, functional-groups, and Ca:P ratio, respectively. Mechanical properties were assessed via 3-point bending and diametral compression. Qualitative microstructural evaluation using scanning electron microscopy (SEM) showed larger pores and a broader pore size distribution (PSD) for materials sintered at 900 ℃ and 1100 ℃, whereas the 1250 ℃ samples showed more uniform PSD. Porosity quantification showed significantly higher porosity for materials sintered to 900 ℃ and 1250 ℃ (p < 0.05). XRD indicated substantial deviations from the 15%/85% HA/β-TCP formulation following sintering where lower amounts of HA were observed when sintering temperature was increased. Mechanical testing demonstrated significant differences between calcination temperatures and different sintering regimes (p < 0.05). Variation in chemical composition and mechanical properties of bioactive ceramics were direct consequences of calcination and sintering.
Keywords: bone graft material; chemical/physical characterization; sintering; bi-phasic calcium phosphate (BCP)
Bioceramics, such as hydroxyapatite (HA) and beta
tri-calcium phosphate (β-TCP), possess two of the ideal characteristics for grafting procedures: osteoconduction and osseointegration . Pure HA has great osteoconductive properties, ability to support the growth of bone over the implant surface, and chemical composition comparable to the inorganic component of bone . HA has a high initial compressive strength,
* Corresponding author. E-mail: email@example.com
Journal of Advanced Ceramics 2013, 2(3): 274–284
but low dissolution kinetics in vivo . Additionally, its slow resorption rates prompted development of more soluble β-TCP ceramics . While it has been shown that β-TCP goes through resorption over a 6–18 month period, it is arguable that it may be too rapid [3,4]. Mixtures of HA and β-TCP ceramic powders have been used to achieve an intermediate solubility and better control of degradation/dissolution rate [5,6].
This study addresses two specific questions with respect to the materials used in grafting processes for boney defects. First is the question of chemistry of the aqueous paste after all processing steps are completed. Is the composition of the ceramic the same as that used to initially formulate the feedstock? More specifically, is there any alteration in the ratio of HA and β-TCP in mixed ceramic scaffolds? The feedstock material is formulated by mechanical mixing of one or two commercially available ceramic powders. The powders are typically pre-processed by calcining at a lower temperature (c.a., 800–1000 ℃) followed by subsequent milling to refine particle size and shape. Then, after fabricating the feedstock and printing, the green ceramic body is subjected to sintering at higher temperatures in a furnace (c.a., 900–1250 ℃) for 4 h.
The second question is addressed: how does processing affect the overall mechanical properties of the resultant ceramic material? The most obvious variables for strength of ceramics are the grain size and flaw (pore) population. Since microporosity, which can be achieved through incomplete sintering, within rods is desirable to a certain extent from a biological function standpoint, what is the overall effect on strength?
While the macroscopic arrangement of lattice-based bioactive ceramic scaffolds (LBBCS) is well controlled through respective fabrication technology and its associated sintering shrinkage [4,7], its chemistry and internal material properties can be significantly altered depending on its composition and subsequent processing steps. For instance, sintering temperature range of β-TCP must be between 1100 ℃ and 1250 ℃, as higher temperatures will lead to its transformation to α-TCP . Sintering temperatures will also affect microporosity, specific surface area, density and porosity, thereby affecting the scaffold’s dissolution properties over time in vivo. Additionally, if high temperatures are utilized, increases in density, grain size, compressive, flexural and torsional strength may be achieved . From a fracture toughness standpoint,
increased levels may be achieved at sintering temperatures between 1100 ℃ and 1150 ℃ while decreased levels have been observed at sintering temperatures higher than 1250 ℃ .
Previous observations and studies regarding bi-phasic calcium phosphate (BCP), which have not concentrated on correlating chemical properties with mechanical properties, have shown that strength among other properties has varied with sintering temperatures [9,10]. Thus, further physicochemical characterization of LBBCS is desirable and will allow further development of such systems for varied clinical applications.
2 Materials and methods
2. 1 Ink preparation
The feedstock, a colloidal gel, which is referred to, as “ink”, was fabricated into cylindrical rods. This colloidal gel was fabricated through a series of powder processing steps beginning with calcining, attrition milling and drying of the individual base materials. HA (Product 10185602, Lot 43640, Honeywell, Germany) was calcined at 800 ℃ or 975 ℃ for 11 h followed by cooling and milling in distilled water for approximately 30 min using an attrition mill (01-Lab Attritor, Union Process, Akron, OH, USA) with a charge of 3 mm diameter zirconia milling media and a mill speed of approximately 120 rpm. The same processing method was used for β-TCP (Product 21218, Lot 1305078, Sigma-Aldrich, Germany) . After milling, the slurry was separated from the milling media and dried in a low-temperature oven (~37 ℃) to yield a dry ceramic powder. The commercially available particle characteristics are unsuitable for ink formulation due to presence of nanoporosity in the particles and a non-equiaxial particle shape. Therefore, it requires calcining and milling processes to remove these limitations and yield a powder suitable for further processing.
After calcining, milling and drying, the colloidal gel was formulated by precise addition of components in a specific order. To produce a 45 ml batch of the colloidal gel, first, ~20 g of 5 mm diameter round zirconia milling media, a pre-calculated amount of distilled water (DI-H2O), and 1.4 g of dispersant molecule (Darvan®821A, R.T. Vanderbilt Company, Inc., Norwalk, CT, USA) followed by appropriately
Journal of Advanced Ceramics 2013, 2(3): 274–284
calculated amounts of HA and β-TCP ceramic powders were added to a 250 ml mixing cup (Thinky Inc., Japan). The mixing cup was placed in a non-contact planetary mixer (model AR-250, Thinky Inc., Tokyo, Japan) for 3 min at 2000 rpm. The cup was then placed in a water bath for ~5 min to cool. Next, an aliquot of hydroxypropyl methylcellulose (Methocel F4M, Dow Chemical Company, Midland, MI, USA) stock solution (5% by weight in water) was added at 7 mg/ml of ceramic and the suspension was again mixed for an additional 2 min at 2000 rpm. The final step was the addition of poly(ethlyenimine) (PEI) (molecular weight = 50–100 kDa, ICN Biomedical, Aurora, OH, USA) as a 10% aqueous stock solution. Initially, 1 ml of PEI solution was added and mixed for 30 s, then PEI solution was added drop-wise followed by mixing until reaching the desired consistency, which when a spatula dragged through the paste leaving a well-defined trench. These characteristics were well described by Smay et al. in previous publications .
2. 2 Methods
2. 2. 1 Sample fabrication Rods of two different HA/β-TCP ratios (volume fraction) were fabricated for evaluating the chemical and physical properties before and after the sintering process. The first sets of samples were compromised of 15%/85% HA/β-TCP colloidal gel. A subsequ